Author
vodien
View
218
Download
0
Embed Size (px)
International Journal of Solids and Structures 6061 (2015) 107124
Contents lists available at ScienceDirect
International Journal of Solids and Structures
journal homepage: www.elsevier .com/locate / i jsols t r
Mechanical response of Ti6Al4V octet-truss lattice structures
http://dx.doi.org/10.1016/j.ijsolstr.2015.02.0200020-7683/ 2015 Elsevier Ltd. All rights reserved.
Corresponding author. Tel.: +1 434 982 5678.E-mail address: [email protected] (L. Dong).
Liang Dong a,, Vikram Deshpande b, Haydn Wadley aa Department of Materials Science and Engineering, University of Virginia, Charlottesville, VA 22903, United Statesb Engineering Department, Trumpington Street, University of Cambridge, UK
a r t i c l e i n f o a b s t r a c t
Article history:Received 11 December 2014Received in revised form 8 January 2015Available online 19 February 2015
Keywords:Octet-truss latticeElastic stiffnessStrengthTitanium alloys
A simple snap-fit and vacuum brazing method has been developed to fabricate three dimensional spacefilling octet-truss lattice structures from Ti6Al4V alloy sheets. Using strut lengths of 725 mm resultedin a relative density of the lattices ranging from 2% to 16%. The lattice elastic stiffness constants andstrengths have been characterized under through-thickness compression and in-plane shear as a functionof their relative density, and are shown to be well predicted by previously proposed micromechanicalmodels adapted to account for the increased nodal mass and strut separations of the snap-fit latticedesign. The Ti6Al4V octet-truss lattices exhibit excellent mechanical properties compared to othercellular material cell topology combinations, and appear to be promising candidates for high tem-perature applications where a robust mechanical performance is required.
2015 Elsevier Ltd. All rights reserved.
1. Introduction
There are many ways to create 3D space filling cellular materials.Periodic cellular structures, are constructed from unit cells withhoneycomb (Bitzer, 1997; Wadley, 2003, 2006; Dharmasena,2008; Russell et al., 2008), tetrahedral (Sypeck, 2002; Kooistra,2004, 2007; Lim and Kang, 2006), 3D Kagome (Lim and Kang,2006; Lee et al., 2007; Park et al., 2011), octet truss (Bitzer, 1997;Fuller, 1961) and pyramidal (Kooistra, 2007; Queheillalt, 2005;Finnegan et al., 2007; Queheillalt et al., 2008) arrangements of websor struts. Tetrahedral, pyramidal and 3D Kagome unit cells requirestruts or webs to connect their out of plane members in order forthem to become statically determinant, stretch-dominated struc-tures (Deshpande et al., 2001). Space filling, structurally efficientlattices can then be constructed by the assembly of these unit cellsin three dimensions. These statically determinate lattice structurescan act as a material in the sense that their properties are indepen-dent of the size of the sample, provided its exterior dimensions arelarge compared to those of its cells. However, in some sandwichpanel applications (Sypeck, 2002; Kooistra, 2004, 2007; Wanget al., 2003) it may be preferable to use only the out of plane websor struts to maintain separation of the face sheets while utilizingthe faces to ensure unit cell static determinacy. Foams made frompolymers, metals or ceramics with interconnected or closed cellsalso provide a means for filling space with a random arrangementof cells (San Marchi et al., 2002). However, their cells have a vari-
able (but low) strut or web nodal connectivity, and are bendingdominated structures with moduli and strengths that decreaserapidly as the fraction of solid material (their relative density) isdecreased (Deshpande et al., 2001).
Lattice structures with open cell intermediate face sheetsbetween the layers of inclined struts, such as the octet-truss lattice(Bitzer, 1997; Fuller, 1961), have attracted considerable recentinterest since they are structurally more efficient than foams of asimilar density made from the same material. Recent castingapproaches have demonstrated the possibility of making octet-truss lattices with strut lengths in the 510 mm range(Deshpande et al., 2001), while self-propagating waveguide or laserbased stereo-lithographic methods, when combined with electro-less nickel plating or vapor deposition have enabled fabricationof micrometer scale structures (Torrents et al., 2012; Zheng et al.,2014; Bauer et al., 2014) offering opportunities to exploit otherfunctionalities of materials available in the small length scale limit.
An octet-truss lattice structure is illustrated in Fig. 1, and wasfirst proposed by Fuller (1961), as a method for filling 3D spacewith a structurally efficient truss structure of arbitrary cell size.Its nodes form a face centered cubic structure, Fig. 1(b). Since thestructure has a high nodal connectivity of 12, its mechanicalresponse is stretch-dominated (Deshpande et al., 2001). Whenmade from high specific modulus and strength materials, theoctet-truss lattice is therefore a weight efficient, stress supportingcellular topology, with a stiffness and strength predicted to scalelinearly with relative density, q (the density of the structure dividedby that of the material from which it is made) (Wadley, 2006).
http://crossmark.crossref.org/dialog/?doi=10.1016/j.ijsolstr.2015.02.020&domain=pdfhttp://dx.doi.org/10.1016/j.ijsolstr.2015.02.020mailto:[email protected]://dx.doi.org/10.1016/j.ijsolstr.2015.02.020http://www.sciencedirect.com/science/journal/00207683http://www.elsevier.com/locate/ijsolstr
Fig. 1. (a) An octet-truss lattice constructed by the 3D packing of unit cells. (b) A unit cell of the face centered cubic crystal symmetry octet-truss lattice is composed of acentral octahedral cell constructed with 12 struts that is bounded by 8 edge tetrahedrons. Each node within the octet lattice lies at the intersection of 12 struts.
Fig. 2. Material property charts comparing material stiffness (a) and strength (b) incompression against density. The experimental data (unit cell response, Table 2)and predicted range of these properties for the Ti6Al4V octet-truss latticestructure fabricated here (Ti6Al4V snap fit octet lattice) have been included forcomparison with other octet lattice truss materials. The grey shaded areas defineregions that cannot be reached under ambient conditions.
108 L. Dong et al. / International Journal of Solids and Structures 6061 (2015) 107124
Material property charts are a useful way to compare themechanical properties of low density materials. Fig. 2 shows thedensity dependent modulus and strength under compressive load-ing for low density foams (polymer, metal and alumina) and spacefilling lattice structures made from investment cast Al7Si0.3Mg(Deshpande et al., 2001), Ti6Al4V and Ti6Al2Sn4Zr2Moalloys (Li et al., 2008a,b), similar structures made by electrodeposi-tion of Ni7P (Torrents et al., 2012; Zheng et al., 2014), from carbonfiber laminate composites (Cheung and Gershenfeld, 2013), photo-sensitive HDDA polymers (Zheng et al., 2014), and by the vapordeposition of alumina (Zheng et al., 2014; Bauer et al., 2014). Themoduli and strengths of both foams and lattices scale with thoseof the materials from which they are made (Gibson and Ashby,1999; Ashby, 2000), but foams are substantially more compliantand weaker than lattice topology counterparts (made with thesame density and material) for reasons identified above.
Octet-truss lattice structures made from low density metalalloys with strut diameters in the millimeter range are potentialcandidates for stress supporting aerospace applications. Light-weight aluminum alloy octet-truss lattice structures have beenmade by an investment casting (Deshpande et al., 2001) and by3D additive manufacturing methods (Rosen, 2007; Chu et al.,2010; Williams et al., 2011). However, these processes remain dif-ficult to implement with the highest strength to weight ratio alloysof aerospace interest. There is particular interest in making octet-truss structures from titanium alloys since their strength to weightratio is approximately twice that of aluminum alloys. Many titani-um alloys can also be used at continuous service temperatures wellabove the limits of other light metal alloys based on aluminum ormagnesium (Kulekci, 2008; Ye, 2003). Some titanium alloys alsohave excellent corrosion resistance, and are therefore widely usedin chemical processing equipment (Couper et al., 2009), and heatexchangers (Lu et al., 1998; Boomsma et al., 2003). The Ti6Al4V alloy is the most widely used titanium alloy, and accounts formore than 50% of total titanium usage. Its uses include aircraft tur-bine engine and structural components, fasteners, high perfor-mance automotive parts, and a variety of marine applications(Boyer et al., 1993; Ritchie et al., 1999; Brewer et al., 1998; Boyerand Briggs, 2005; Froes et al., 2004; Gorynin, 1999).
Titanium alloy lattice structures have been fabricated withaerospace-quality investment casting techniques (Li et al.,2008a,b). While this approach has the potential to enable fabrica-tion of complex shaped structures, it is costly to implement, andrequires development of methods to detect and repair the castingdefects often present in investment cast lattice structures (Wanget al., 2003). Because of the cost and complexity of the titaniuminvestment fabrication process, there is very limited mechanical
property data for titanium-based lattice structures as a functionof their relative density, Fig. 2.
L. Dong et al. / International Journal of Solids and Structures 6061 (2015) 107124 109
Here, we explore the use of a simple snap-fit method(Finnegan et al., 2007) for fabricating the struts and open facesheets of planar octet-truss structures from thin plate material.This assembly method is combined with vacuum brazing tofabricate octet-truss lattices from a Ti6Al4V alloy sheet. Themechanical responses of the titanium octet-truss lattices undercompression and shear have been experimentally investigated,and their compressive and shear strengths and moduli determinedas a function of lattice density, and compared with microme-chanical predictions to evaluate the inter relationships betweenlattice topology, material properties and relative density.
2. Lattice fabrication, relative density and solid materialproperties
2.1. Lattice fabrication
The octet-truss lattice structures were fabricated from Ti6Al4V sheets of a single thickness, t = 1.59 mm, in a three step processsummarized schematically in Fig. 3. The truss row patterns,Fig. 3(a), and intermediate (open cell) face sheets, Fig. 3(c), werewater jet cut from as-received Ti6Al4V sheets forming thegeometries shown in the two figures. Rows of trusses werecollinearly aligned and a second collinear array, oriented at 90to the first, was snap-fit attached to their tops forming a [0/90]arrangement of trusses enclosing a pyramidal void shape,Fig. 3(b). Control of the slot tolerance in the nodal regions enableda mechanically stable snap-fitted plane of pyramidal trusses to beassembled in this way. The truss layer planes were then snap-fittedinto the crosses of the intermediate face sheet and the processrepeated to form the octet-truss lattice, Fig. 3(d). Samples withsquare cross section trusses of width t, and various lengths, l, weremade to enable study of the truss slenderness ratio, t/l, uponmechanical response. The geometric parameters defining thestructures assembled for testing are defined in Fig. 4 and their val-ues summarized in Table 1 for each test structure. The maximumgap (determined by the tolerances of the water-jet cutting process)between struts meeting at the nodes was about 90 lm.
The snap-fit lattice was bonded using a vacuum brazingapproach. A 40Ti20Cu20Ni20Zr (wt.%) braze alloy (Lucas Mil-haupt) was first applied to the nodal regions of the assembledstructure. The alloy was applied as a powder carried in a polymerbinder. Brazing was accomplished by placing the lattice structuresin a high-temperature vacuum brazing furnace and heating at10 C/min to 500 C, holding for 20 min to volatilize and removethe polymer binder from the furnace, and then heating to 900 Cfor 30 min at a chamber pressure of 5 102 Pa. This braze alloyhas a solidus temperature of 848 C. Once melted, it wetted thistitanium alloy well, and flowed freely to fill small gaps at the nodesat the brazing temperature used in the study. After brazing, thefurnace was cooled at a rate of 45 C/min, to 600 C, at which tem-perature a 20 min annealing was performed to reduce internalresidual stress. The furnace was finally cooled to ambient tem-perature at a rate of 15 C/min.
The strength of a brazed bond between two plates generallydecreases as the gap between them increases. Lap shear test cou-pons with gaps of 90 lm were included in the brazing runs andsubsequently tested, in accordance with the ASTM D1002 standard,to ensure adequate bond strength was achieved. The measuredshear strength of 40Ti20Cu20Ni20Zr bonded Ti6Al4V sheetswas found to be approximately 450 MPa for a brazed joint gap ofabout 90 lm.
Photographs taken from several orientations of one of thebrazed lattice structures later used for compression testing areshown in Fig. 5. Octet-truss lattice structures for shear testing werealso manufactured with solid external face sheets to facilitate grip-
ping in a shear test fixture. Since the in-plane shear response of theoctet-truss core is anisotropic, the response is dependent on thedirection of shearing. The unit cell sketched in Fig. 4(c) specifiesthe shearing direction by the angle, a = 45 or 0. Photographs ofthe shear samples for testing in both a = 45 and 0 orientationsare shown in Fig. 6 during their assembly process so that the orien-tation of the lattice can be clearly seen. The top row of photographsshows that a two cell wide, octet-truss core, orientated witha = 45 can have either two or three nodal connections with thesolid face sheet through which shear loads were applied. Sincethe number of nodal connections at the edge of a shear sampleinfluences the mechanical response, samples with two edgegeometries (identified as Type I and II), were fabricated, and alsoshown at various stages of assembly in Fig. 6(a) and (b).
2.2. Relative density
A schematic drawing of the octahedral unit cell of the snap-fitlattice is shown in Fig. 4(c) together with coordinate systems usedlater. It also defines the geometric parameters of the lattice. Notethat for the square cross section truss, t = w, and we selected a trussinclination angle x = 45 to balance the compressive and shearresponses of the structure. By calculating the volumes of regionsoccupied by material, and scaling this by the unit cell volume,the relative density, q of the octahedral unit cell of the snap-fitoctet-truss lattice (including nodal mass contributions) is given by;
q 6ffiffiffi2p
lt2 K1 K2t 2ffiffiffi2p
t2
t
l K3l K421
where,
K1 ffiffiffi2pb 2m2 2
ffiffiffi2p
hb c 4ffiffiffi2p
bhtab
K2 2ffiffiffi2p 2b 2c 2
ffiffiffi2ph htab 8m
K3 ffiffiffi2ph 2htab;
K4 ffiffiffi2p
2b c
and the geometric parameters are defined on Fig. 4.Eq. (1) was arranged in this way to separate volume contribu-
tions from the trusses (first term of the numerator) and nodes.Some further simplification can be achieved by introducing non-di-mensional lengths; t t=l, b b=l, c c=l; htab htab=l, h h=l andm m=l. As a result, K1 K1=l2, K2 K2=l, K3 K3=l, andK4 K4=l, whereupon;
q 6ffiffiffi2p
t2 K1 K2t 2ffiffiffi2p
t2
t
1 K31 K42 2
It can be shown that in the limit of vanishing node size, Eq. (1)reduces, in a first order approximation, to the relative densityexpression for the ideal octet-truss lattice;
qoct 6ffiffiffi2p t
l
23
Octet-truss lattice structures, with the extra mass of nodal mate-rial accounted for, have a relative density given by Eq. (1), and werefabricated with relative densities ranging from 2% to 16% by allow-ing the strut length l to vary between 7 and 25 mm. All the latticestructures had square cross section struts with a width, w and thick-ness t = 1.59 mm, and node widths defined by b = 4.76 mm and
Fig. 3. Schematic illustration of the snap-fit truss fabrication and assembly method for making the Ti6Al4V octet-truss lattice.
110 L. Dong et al. / International Journal of Solids and Structures 6061 (2015) 107124
c = 2.24 mm. The relative densities calculated by either Eq. (1) (or byEq. (3)) ranged from 2.4% (or 3.4%) for the lowest density sample to15.9% (or 43.3%) for the highest density sample.
2.3. Solid material characterization
A low magnification micrograph of the nodal region of a brazedlattice structure taken in the backscattered electron imaging (BSE)mode1 is shown in Fig. 7(a). It can be seen that the braze alloy wet-ted the Ti6Al4V base metal and was drawn into both the narrowand wider gaps between the truss members. High magnificationviews of both narrow and wider gap areas, marked by dashed boxesin Fig. 7(a) at the central bond line are shown in Fig. 7(b) and (c).Since the brazing temperature (900 C) was below the b-phase tran-sus temperature (980 C) for the Ti6Al4V alloy (Donachie, 2000),the original equiaxed a-grain and intergranular b-phase microstruc-ture of the original alloy was preserved. The average grain diameterof the a-phase was about 7 lm, while the average thickness of theb-phase was less than 1 lm, Fig. 8.
A brazed joint typically consisted of three zones marked 1, 2and 3, Fig. 7(b). Region 1 was the diffusion zone with a fineWidmansttten structure in the base alloy near the interface(Onzawa et al., 1990; Botstein and Rabinkin, 1994; Lugscheiderand Broich, 1995). Region 2 was a b-titanium rich zone next tothe diffusion zone, while region 3 was a brittle intermetallic phaserich zone at the center of the braze filled region (at center ofFig. 7(b)). The central (brittle intermetallic phase rich) zone couldbe eliminated when the brazing joint clearance was sufficientlysmall, as shown in Fig. 7(c). In this case, the brazed joint consistedof only the diffusion and b-titanium phase zones with a totalthickness of approximately 90 lm. Elemental distribution maps
1 Lighter grey contrast regions correspond to areas with a higher concentration ofhigh atomic number elements.
corresponding to regions (b) and (c) of Fig. 7 are shown inFig. 7(d) and (e) respectively. They show the spatial distributionof the alloy elements (Ti, Al, V) and those of the braze alloy(Zr, Ni, and Cu) for both the narrow and wide gap regions of a brazejoint. Substantial lateral diffusion of Zr, Cu and Ni into the titaniumalloy had occurred in the narrow clearance region of a joint. How-ever, the intermetallic rich region at the center of the wider gapregions of a joint retained substantial Cu, Zr and Ni from the brazealloy following the brazing recipe used here.
In order to later predict lattice mechanical properties, the uni-axial tensile response of Ti6Al4V alloy subjected to the samethermal history as the lattice structures was measured. The tensileresponse measured at a strain rate of 104 s1 is shown in Fig. 9.The elastic (Youngs) modulus, Es and 0.2% offset yield strength,rys were 123 GPa and 932 MPa, respectively. The tangent modulus,Et (given by the slope of the true stresstrue strain response of thesolid material at the inelastic bifurcation stress, rIE) was obtainedby differentiation of a modified RambergOsgood fit (Rasmussen,2003) to the measured stressstrain responses. The inelastic bifur-cation stress was obtained using the tangent modulus theory (Gereand Timoshenko, 1984; Shanley, 1967) as discussed in Section 4.2.
3. Compression and shear responses
The Ti6Al4V octet-truss lattices were tested at ambient tem-perature in free compression and shear at a nominal strain rate of3 104 s1 in accordance with ASTM standards C365 and C273.The ASTM C273 standard specifies use of a compression shear plateconfiguration and a length to thickness ratio of the shear sandwichpanel larger than 12:1; however, a smaller length to thickness ratiois also acceptable as later clarified by Adams (Adams, 2007). Theshear samples used here had a length to thickness ratio of about4:1. The shear response was also dependent upon the directionof loading with respect to the lattice orientation. Tests were
Fig. 4. The geometries with relevant design variables identified of (a) the out ofplane trusses and (b) the intermediate truss layer, (c) the unit cell of the snap-fitmodified octet-truss lattice with the Cartesian co-ordinate system and loadingdirections also specified.
L. Dong et al. / International Journal of Solids and Structures 6061 (2015) 107124 111
therefore conducted at two orientations to determine the twoindependent in-plane shear tensor strength and moduluscomponents. The measured load cell forces were used to calculatethe compressive and shear stresses applied to the structure. The
Table 1Node and strut dimensions for the octet-truss lattices used in this study (unit: mm).
t w b c h
1.588 1.588 4.763 2.235 0.953
sample side lengths are defined using Figs. 5 and 6, as the distancesbetween the left-and-right edges of the samples while the top-and-bottom edges were defined by the out-of-plane edge struts.The volume occupied by the extra edge nodes was not taken intoaccount since they contribute neither stiffness nor strength (theycould be trimmed off if necessary without changing the mechani-cal response). The loading directions are shown in Fig. 4(c). A laserextensometer measured the compressive strain by monitoring thedisplacements of the top and bottom perforated intermediate sur-face layers, and the shear strain by monitoring the displacementsof the shear plates. Unloadingreloading cycles were conductedprior to the onset of inelastic deformation in order to determinethe elastic stiffness components of the specimens.
3.1. Compression results
The z (through-thickness) direction compressive stressstrainresponses of the lattice structures are shown in Fig. 10. The respon-se exhibited characteristics typical of cellular structures including;a region of nominally elastic response, yielding, plastic strain hard-ening to a peak in strength, followed by a drop in flow stress to aplateau region and finally rapid hardening associated with contactof the deformed struts with each other (densification). In contrastto many foam topology materials, the drop in flow stress afterattainment of lattice strength was very large, and indicative of amechanical instability. Photographs of the lattice structures show-ing characteristic plastic deformation behaviors in compression areshown in Fig. 11.
The lowest relative density lattice (q 2:4%) failed by elasticbuckling of the struts. Higher density samples failed by inelasticbuckling or yielding of the out-of-plane strut members as thelattice strength was achieved. The out-of-plane struts continuedto buckle with increasing plastic strain, which resulted inincreased deflection of the struts and asymmetrical loading atthe nodes which caused nodal rotation. Strut buckling wasaccompanied by a significant drop in flow stress. The in-planestruts were also subjected to torsion and bending deformationsdue to nodal rotations. Lateral (Poisson) expansion of the latticeswas also observed during compression without a lateral bound-ary constraint. Plastic hinges were formed near the middle andtwo ends of the out-of-plane struts. Truss fracture was finallyobserved at the plastic hinges of the out-of-plane struts, andfor in-plane struts near their nodal connections due to the sig-nificant deformation induced by the combined tension, bendingand torsion loading in these regions. The buckled trusses eventu-ally contacted each other at the densification strain coincidentwith rapid hardening of the flow stress versus strain curve. Itis noted here that the flow stress dropped quickly after the peakin strength, which indicates less than the ideal energy absorp-tion seen in some other structures (San Marchi et al., 2002;Gibson and Ashby, 1999; Holloman et al., 2013). This effect isattributed to the buckling instability of struts made from a lowstrain hardening rate (tangent modulus) Ti6Al4V alloy. Table 2summarizes the relative densities (calculated using Eq. (1)), t/lratios, elastic compressive moduli and compressive strengths ofthe octet-truss lattice compression specimens.
The octet truss does not have long range buckling modes and sowe expect the one layer structure to give representative results forthe peak strength. However, post-peak collapse bands may be
htab x t0 m R
1.588 45 1.270 1.346 5.080
Fig. 5. Photographs of a Ti6Al4V octet-truss lattice compression specimen with a relative density of 4.6%; (a) view in the compression loading direction, (b) a side viewshowing the out-of-plane pyramidal struts and (c) an isometric view. (d) Shows a close-up of a brazed node at the side of the sample where three struts from above and belowmeet two of the intermediate layer at a sample edge node.
Fig. 6. Photographs of octet-truss shear test structures with a relative density of 10.4%. (a) Corresponds to a Type I sample subsequently loaded at a = 45, (b) to a Type IIsample also loaded at a = 45 and (c) is a sample to be tested at a = 0. Photographs of the corresponding disassembled parts before brazing are used to illustrate the internaltruss structures.
112 L. Dong et al. / International Journal of Solids and Structures 6061 (2015) 107124
affected by the specimen size employed and will require investiga-tion in future studies.
3.2. Shear results
The (001) in-plane shear stressstrain responses of the latticestructures are shown in Fig. 12 for a = 45 and 0. For test orienta-tions with a = 45, each unit cell has four out-of-plane strut mem-
bers loaded in compression and four in tension; whereas, in thecase of shear loading in the a = 0 direction, a unit cell has onlytwo out-of-plane strut members loaded in compression and twoin tension. The a = 45 samples were fabricated to investigate theeffect of the edge nodal connectivity. The Type I samples had a con-cave edge truss geometry, Fig. 12(a), while that of the Type II coreswas convex, Fig. 12(b). It is evident that an end nodal deflection inthe z (through-thickness) direction will occur for a = 45 Type II
Fig. 7. (a) Cross-sectional SEM image (in BSE contrast mode) through a brazed node. Higher magnification views of the rectangular areas A and B are shown in (b) and (c)respectively. Elemental composition maps are shown for region A in (d) and for region B in (e).
Fig. 8. Microstructure within the Ti6Al4V struts after the brazing heat treatment(900 C, 30 min). The a-phase grain size was approximately 7 lm.
Fig. 9. True tensile stressstrain response of the Ti6Al4V alloy after exposure tothe thermal cycle used for brazing. A modified RambergOsgood fit to the stressstrain response is also shown. The tangent modulus as a function of strain (obtainedas the derivative of the modified RambergOsgood curve) is also overlaid on thedata.
L. Dong et al. / International Journal of Solids and Structures 6061 (2015) 107124 113
cores and for a = 0 cores under (001) in-plane shear loading.However the end nodes of a = 45 Type I cores are stable under(001) in-plane shear loading.
Most of the samples exhibited stress versus strain responsestypical of lattice sandwich cores including elastic behavior duringinitial loading followed by work hardening until the lattice shearstrength was achieved. However, the lowest density sample(q 2:4%) failed by elastic buckling of the out-of-plane struts atthe peak in flow stress. Samples with higher relative densities ini-tially failed by inelastic buckling or tensile yielding of the out-of-plane struts. Continued loading eventually resulted in fracture ofthe tensile loaded truss members near their nodes when the latticeshear strength was reached. This was accompanied by an abruptdrop in flow stress. Plastic buckling of some out-of-plane trussmembers at the ends of the shear samples was observed prior to
attainment of the lattice shear strength. This was a manifestationof the compressive loading component of the ASTM C273 testmethod. Deflection of the edge nodes at the two ends of the shearsamples was observed in the cases of a = 0 and 45 Type II. Suchan edge effect is attributed to the lack of loading symmetry, whichresulted in a z (through-thickness) direction force at these endnodes. The relative densities (calculated using Eq. (1)), t/l ratios,
Fig. 10. Compressive stressstrain responses of snap-fit Ti6Al4V octet-trusslattice samples with different relative densities.
114 L. Dong et al. / International Journal of Solids and Structures 6061 (2015) 107124
elastic shear moduli and shear strengths of shear samples are sum-marized in Tables 35.
4. DFA and generalized models for octet-truss lattice
The mechanical properties of the ideal octet-truss latticematerial (attained in the limit of vanishing node volume) havebeen analyzed by Deshpande et al. (2001). This DFA modelexamined an ideal octahedral cell, and the results apply to the
Fig. 11. Photographs of (a) the (100) and (b) the (110) planes of a lattice with q 4:6%total strain, e, increased.
octet-truss lattice constructed by a 3-D stacking of such octahedralunit cells. It was shown that for small t/l, the contribution to overallstiffness of the octet-truss lattice from the bending of the struts wasnegligible compared to that from strut stretching. The DFA modelassumed pin-joined struts, and applied a first order approximation
to the relative density with the form qoct 6ffiffiffi2p
tl
2 (Eq. (3)) whichslightly overestimates the relative density due to a double countingof the small nodal volume. The DFA model assumed the octahedralcell had a face-centered-cubic symmetry; there are three indepen-dent elastic compliance constants, Sij (the contracted indices i and jare ordered pairs of Cartesian indices) for a cubic system, i.e., theset {Sxxxx, Sxxyy, Syzyz} (equivalent to {S11, S12, S44} with contractedindices), and the linear elastic strain, ei and stress, rj tensor relation-ship took the form (with Cartesian indices);
exxeyyezzeyzexzexy
2666666664
3777777775
Sxxxx Sxxyy Sxxyy 0 0 0Sxxyy Sxxxx Sxxyy 0 0 0Sxxyy Sxxyy Sxxxx 0 0 0
0 0 0 Syzyz 0 00 0 0 0 Syzyz 00 0 0 0 0 Syzyz
2666666664
3777777775
rxxryyrzzryzrxzrxy
2666666664
3777777775
4a
where the components of elastic compliance matrix are given by;
Sxxxx Sxxyy Sxxyy 0 0 0Sxxyy Sxxxx Sxxyy 0 0 0Sxxyy Sxxyy Sxxxx 0 0 0
0 0 0 Syzyz 0 00 0 0 0 Syzyz 00 0 0 0 0 Syzyz
2666666664
3777777775 1
qoctEs
9 3 3 0 0 03 9 3 0 0 03 3 9 0 0 00 0 0 12 0 00 0 0 0 12 00 0 0 0 0 12
2666666664
37777777754b
during compression. The development of inelastic truss buckling can be seen as the
Table 2Relative densities, t/l ratio, experimental and unit cell compressive moduli and strengths of the manufactured snap-fit Ti6Al4V octet-truss lattice compression specimens. Therelative densities were calculated using Eq. (1).
Strut length(l, mm)
t/l Relativedensity (q) (%)
Sample compressivestiffness (GPa)
Unit cell compressivestiffness (GPa)
Sample compressivestrength (MPa)
Unit cell compressivestrength (MPa)
Energy absorption per unitvolume, Wv (MPa)
25.400 0.063 2.4 0.49 0.39 4.2 3.5 0.5216.891 0.094 4.6 0.97 0.78 14.1 11.9 2.9912.014 0.132 7.8 2.04 1.64 26.3 22.5 6.119.728 0.163 10.4 2.69 2.16 35.7 30.8 9.528.433 0.188 12.6 3.49 2.81 44.2 38.4 12.247.010 0.226 15.9 4.94 3.98 56.5 49.4 21.16
L. Dong et al. / International Journal of Solids and Structures 6061 (2015) 107124 115
where Es refers to the Youngs modulus of the strut material. Theprincipal material axes, as shown in Fig. 4(c), are defined as a Carte-sian co-ordinate system for the analysis.
4.1. Stiffness predictions
The DFA model (Deshpande et al., 2001) predicts the z ([001]through-thickness) direction Youngs modulus;
Ezz REel qoctEs 19
qoctEs 5
where REel is the elastic compressive modulus coefficient with a val-ue of 1/9, qoct is the relative density given by Eq. (3), and Es is theYoungs modulus of the solid material from which the lattice was
constructed. The relative compressive modulus, EzzEs 2ffiffi2p
3tl
2, is lin-early related to the elastic compressive modulus coefficient andthe ideal octet relative density, qoct.
The (001) in-plane shear modulus is given by;
Gzx RGel qoctEs 1
12qoctEs 6
where RGel is an elastic shear modulus coefficient with a value of
1/12, and the relative (001) in-plane shear modulus is GzxEs ffiffi2p
2tl
2.The relative shear modulus, GzxEs is therefore linearly related to the
elastic shear modulus coefficient, RGel, and the ideal octet relativedensity, qoct. The cubic symmetry dictates that the (001) in-planeshear modulus is independent of the shear direction in this plane.
The DFA model predicts density independent (constant) elastic
stiffness coefficients REel and RGel
; a consequence the DFA models
analysis of an ideal octahedral cell without the nodal volume ofreal samples taken into account. This can be addressed using thefree body diagram method (Finnegan et al., 2007), which showsthat the total external force required for each individual strut toachieve an identical state of strain is a constant. As shown inAppendix B, the elastic modulus coefficient, Rel, is linearly relatedto the specimens octahedral cell height (H), its cross-section area(A), and the relative density q now given by Eq. (1);
Rel KelH
lAq7a
The relative compressive modulus is then given by;
EzzEs REel q K
Eel
HlA
7b
The relative (001) in-plane shear modulus is given by;
GEs RGel q K
Gel
HlA
7c
where Kel is a constant with KEel 23 t
2 for the compressive modulus
coefficient, and KGel 12 t2 for the (001) in-plane shear modulus coef-
ficient. The specimen octahedral cell height (H), its cross-sectionalarea (A) and the relative density (q) are all now functions of thenodal geometry of the lattices tested here.
In the limiting DFA model case, H ffiffiffi2p
l, and A l2, and thecompressive modulus coefficient, relative compressive modulus,shear modulus coefficient, and relative shear modulus given by
Eq. (7) reduce to 19,2ffiffi2p
3tl
2, 112, and ffiffi2p2 tl 2 respectively (i.e. the DFAmodel predictions). Eq. (7) is subsequently referred to as a gener-alized octet-truss lattice elastic modulus model which can be usedto analyze the snap-fit octet-truss lattice whose struts do not makecontact at a node (non-zero values of b, c, h, htab, m, in Fig. 4) andtherefore contains extra nodal mass.
4.2. Strength predictions
4.2.1. Compressive strengthA stretch dominated cellular lattice may collapse under com-
pressive loading by elastic or inelastic buckling, or by plastic yield-ing depending on the slenderness (t/l ratio for a solid strut oflength l and square cross section of side length t) of the struts.
At high relative densities, l tends towards t, and a lattice will failby yielding of the low aspect ratio struts. Lattice strength, rpk thenlinearly scales with the yield strength, rys of the solid material, andthe load bearing area (i.e. relative density, q) of the lattice;
rpk rys qRr 8
where Rr is a lattice topology (strut orientation) dependentstrength coefficient (Wadley, 2006).
At low densities, struts are slender enough to collapse by elasticbuckling prior to compressive plastic yielding, and lattice strengthis obtained by replacing the strut material yield strength, rys in Eq.(8), with the elastic buckling stress given by;
rE k2p2EsI
Al2 k
2p2Es12
tl
29
where I is the second moment of area of the strut, A is the strutcross-sectional area (I t412 ; A t
2, for a solid strut with squarecross section of side length t) and the factor k is determined bythe end conditions on the buckling struts. If the ends of the strutsare pin-jointed, and can freely rotate k = 1 while selection of k = 2corresponds to a strut whose ends are buried and cannot rotate dur-ing buckling.
At intermediate relative densities, buckling occurs after thestress in the strut has exceeded the proportional limit of the solidmaterial, but before the stress attains the ultimate strength of thesolid. In this case, the compressive strength of the lattice is con-trolled by inelastic buckling at an inelastic bifurcation stress givenby the tangent modulus theory (Gere and Timoshenko, 1984;Shanley, 1967). In this case the compressive strength is found byreplacing Es in Eq. (9) by the tangent modulus Et at an inelasticbifurcation stress level, i.e., by replacing rE with rIE given by:
Fig. 12. Shear stressstrain responses for (a) Type I and (b) Type II Ti6Al4V octet-truss lattice shear specimens of different relative densities loaded in the a = 45 direction.Lattice responses when loaded in the a = 0 direction are shown in (c). Photographs revealing the failure modes are also shown for Type I (d) Type II (e) and a = 0 (f) shearsamples all with q 4:6%.
116 L. Dong et al. / International Journal of Solids and Structures 6061 (2015) 107124
rIE k2p2EtI
Al2 k
2p2Et12
tl
210
The DFA model for the ideal octet-truss lattice assumed thestrut material to be elastic-perfectly plastic with a tangent modu-lus of zero; therefore the only mechanisms for lattice failure wereelastic buckling and plastic yielding. In the case of an ideal octet-truss lattice with a vanishing node size, and with the principal axesdefined as shown in Fig. 4(c), the DFA model Deshpande et al., 2001predicts the z (or [001]) direction compressive strength when theelastic buckling failure mechanism is operative;
rpkzz p2Es36
qocttl
211
The DFA model assumes k = 1 for the end conditions of thestruts, though the precise value is likely to be influenced by thenode design and the mechanical properties of the solid materialused to make the structure.
In the case of plastic yielding governed failure;
rpkzz 13
qoctrys 12
Table 3Relative densities, t/l ratio, experimental and unit cell shear moduli and strengths ofthe manufactured snap-fit Ti6Al4V octet-truss lattice shear specimens (a = 0). Therelative densities were calculated using Eq. (1).
Strutlength(l, mm)
t/l Relativedensity(q) (%)
Sampleshearstiffness(GPa)
Unit cellshearstiffness(GPa)
Sampleshearstrength(MPa)
Unit cellshearstrength(MPa)
25.400 0.063 2.4 0.35 0.28 2.3 1.916.891 0.094 4.6 0.69 0.55 6.7 5.612.014 0.132 7.8 9.728 0.163 10.4 1.88 1.48 16.9 14.38.433 0.188 12.6 7.010 0.226 15.9 3.60 2.84 28.5 24.4
L. Dong et al. / International Journal of Solids and Structures 6061 (2015) 107124 117
For a material with a non-zero tangent modulus, the inelasticbuckling criterion can be simply obtained by replacing Es in Eq.(11) with Et, to give;
rpkzz p2Et36
qocttl
213
In Eqs. (11)(13), qoct refers to that given by Eq. (3).The snap-fit octet-truss lattice structures fabricated here have a
considerable node volume and struts ends are laterally separatedwhich requires the nodal geometry to be explicitly addressed.Since the total external force required for each individual strut toachieve an identical state of strain is a constant, a more generalexpression for the compressive strength coefficient (Rr), assumingpin-joined struts (k = 1), as a function of the specimen octahedralcell cross-sectional area, A and relative density, q was derived inAppendix B;
Rr KrrcAq
14a
and the relative compressive strength is defined as
rpkzzrys Rr q Kr
rcA
14b
where Kr is a constant 2ffiffi2p
t2rys and rc refers to the collapse strength
of a single strut, given by rys in the case of the plastic yielding fail-ure mode or the critical buckling stresses given by Eqs. (9) and (10)for the corresponding buckling failure modes, and q in Eq. (14) isthat defined in Eq. (1). It can be shown that in the limit of vanishingnodal volume, Eq. (14) reduces to the DFA model prediction (Eqs.(11)(13)).
4.2.2. The (0 0 1) in-plane shear strengthThe (001) in-plane shear strength depends on the shear loading
direction in the plane. For a 0, the measured shear strength spk0is spkzx, with the principal axes defined as shown in Fig. 4(c). The DFAmodel for an ideal octet-truss lattice with vanishing node volume
Table 4Relative densities, t/l ratio, experimental shear moduli and strengths of themanufactured snap-fit Ti6Al4V octet-truss lattice shear specimens (a = 45, TypeI). The relative densities were calculated using Eq. (1).
Strut length(l, mm)
t/l Relative density(q) (%)
Shear stiffness(GPa)
Shear strength(MPa)
25.400 0.063 2.4 0.31 2.616.891 0.094 4.6 0.61 8.512.014 0.132 7.8 1.14 15.79.728 0.163 10.4 1.76 21.08.433 0.188 12.6 2.33 26.77.010 0.226 15.9 2.56 34.4
predicts (Deshpande et al., 2001) that failure by elastic bucklingresults in a lattice shear strength given by;
spk0 spkzx p2Es72
qocttl
215
For failure by plastic yielding;
spk0 spkzx 16
qoctrys 16
When failure occurs by inelastic buckling;
spk0 spkzx p2Et72
qocttl
217
In Eqs. (15)(17) qoct is that defined in Eq. (3).In the case of a 45, the measured shear strength, spk45 , of the
ideal octet-truss lattice when failure occurs by elastic buckling isgiven by;
spk45 ffiffiffi2p
p2Es72
qocttl
218
When failure occurs by plastic yield, the shear strength is;
spk45 ffiffiffi2p
6qoctrys 19
While for inelastic buckling, the shear strength is given by;
spk45 ffiffiffi2p
p2Et72
qocttl
220
Eqs. (18)(20) are DFA model predictions, and qoct thereforerefers to that given by Eq. (3).
A more general expression for the (001) in-plane shear strengthcoefficient (Rs) of the snap-fit octet-truss lattice can be written as afunction of the specimen cross-sectional area, A and relative densi-ty, q (see Appendix B);
Rs KsrcAq
21a
While the relative (001) in-plane shear strength is;
srys Rs q Ks
rcA
21b
where Ks is a constant. For a 0, Ks ffiffi2p
t2rys while for a 45
,
Ks 2t2
rys , if it is assumed that the struts are pin-joined. In Eq. (21),q now refers to that given by Eq. (1).
5. Comparison of predictions with measurements
Before comparisons between the measured and modeled prop-erties of the snap-fit lattice can be made, it is necessary to adjustthe measured properties of the compression, Fig. 5(c) and a 0shear samples, Fig. 6(c), to account for edge struts that belong to
Table 5Relative densities, t/l ratio, experimental shear moduli and strengths of themanufactured snap-fit Ti6Al4V octet-truss lattice shear specimens (a = 45, TypeII). The relative densities were calculated using Eq. (1).
Strut length(l, mm)
t/l Relative density(q) (%)
Shear stiffness(GPa)
Shear strength(MPa)
25.400 0.063 2.4 0.22 2.016.891 0.094 4.6 0.41 6.212.014 0.132 7.8 9.728 0.163 10.4 1.07 15.68.433 0.188 12.6 7.010 0.226 15.9 1.89 25.6
Fig. 13. Comparisons between the measured and model predicted relative elastic moduli (normalized by solid material modulus) as a function of (t/l)2 and relative density qfor the snap-fit lattice. The corresponding predictions of the DFA model (which assumes a vanishing node volume) and the generalized octet-truss lattice model (whichaccounts for the nodal separation and additional nodal mass of the snap-fit structure) are shown in (a) and (c) as a function of the strut aspect ratio. Generalized latticemodel is the abbreviation of generalized octet-truss lattice model.
118 L. Dong et al. / International Journal of Solids and Structures 6061 (2015) 107124
the unit cells of a larger area sample. These edge struts of partialunit cells contribute both stiffness and strength to the samplesmechanical response. If it is assumed the edge struts of adjacentcells behave in the same manner as their inner strut counterparts,the total force required to deform the counterpart lattice withoutredundant edge struts can be shown (by taking the ratio of thenumber of out-of-plane struts that contribute stiffness/strengthin lattices without extra edge struts to the total number of out-of-plane struts in the tested samples. All the out-of-plane strutscontribute stiffness/strength for compression samples, whereasonly the 0 orientated out-of-plane struts are taken into accountfor the a 0 shear samples) to be 4/5 that of the snap-fit latticesamples actually tested. The strength of a lattice without extraedge struts is then given by this applied force divided by itscross-sectional area, and is subsequently defined as the unit cellstrength; the unit cell stiffness is then obtained as this stress divid-ed by the imposed strain. It is noted here that the manufacturedsamples have a height of H + t; whereas, the octahedral cell asshown in Fig. 4(c) has a height of H. Tables 2 and 3 summarizethe sample and unit cell moduli and strengths of both the compres-sion and a 0 shear lattice samples. Since there are no redundantout-of-plane edge struts in the a 45 shear lattice samples testedhere; the definition of unit cell stiffness/strength was not used inthe a 45 case.
The mechanical properties of a lattice reviewed in Section 4, area function of its number and orientation of struts and the strut t/lratio, as well as strut material mechanical properties. The nodes
are parasitic mass which do not change the strut response, as longas k, the factor accounting for the rotational stiffness of the trussends, is not affected. The unit cell elastic moduli for compression
and a 0 shear samples are therefore plotted against tl 2, in
Fig. 13(a) and (c), and the relative compressive and shear strengths
against tl 2 in Figs. 14(a) and 15(a) and (c) since this abscissa scales
with the relative density of both an ideal octet-truss lattice and thesnap-fit structure. The DFA model predictions are overlaid on theseresults. The elastic moduli are also plotted against the snap-fitstructures relative density, q, which includes the parasitic nodalmass (as given by Eq. (1)), in Fig. 13(b) and (d), and the strengthdata in Figs. 14(b) and 15(b) and (d). Generalized octet-truss lattice
model predictions are plotted against both tl 2 and the snap-fit
structures relative density, q, which takes into account the extranodal volume, on all the figures.
The relative elastic moduli (Ezz=Es and G=Es) for the snap-fit Ti6Al4V octet-truss lattice structure deduced from the measuredunit cell relative elastic moduli for compression and a 0 shearsamples are shown in Fig. 13 as a function of tl
2 and the snap-fit structures relative density q. Examination of Fig. 13(a) and (b)shows that the compressive modulus data is over predicted bythe DFA model but is in excellent agreement with the generalizedoctet-truss lattice model which accounts for actual nodal geometryof the tested samples. Fig. 13(c) and (d) show three sets ofexperimental data for the relative shear moduli measured ata = 0, and for both the Type I and II shear structures tested at
L. Dong et al. / International Journal of Solids and Structures 6061 (2015) 107124 119
a = 45. It is evident that the DFA model is unable to predict thesnap-fit structures responses; a consequence of the strut separa-tion at the nodes. By taking into account the nodal geometry, thegeneralized octet-truss lattice model predictions agree well withthe a = 45 Type I and a = 0 measurements. However, the general-ized shear modulus model is still unable to predict the a = 45 TypeII structure response as well. In the DFA model, nodal rotationsduring shear loading were constrained by symmetry during theanalysis. In the a = 45 Type II case experiments, insufficient nodalconnectivity at the end nodes of the finite length samples led tosubstantial nodal rotation, Fig. 12(e). The edge struts connectingthese end nodes then made a reduced (negligible) contribution tothe core stiffness since they underwent little axial (stretching)deformation. If the stiffness contribution from the edge struts con-necting the end nodes (a quarter of the struts) is neglected, theshear stiffness of the as manufactured a = 45 Type II core wouldbe approximately 3/4 (by taking the ratio of the number of out-of-plane struts that contribute stiffness to the total number ofout-of-plane struts in the tested a = 45 Type II shear samples) thatof a = 45 Type I core. The generalized octet-truss lattice shear stiff-ness model prediction for the a = 45 has been multiplied by 3/4,and is shown to then be in good agreement with the a = 45 Type
II measurement when plotted against tl 2 in Fig. 13(c) or the snap-
fit structures relative density in Fig. 13(d).The relative unit cell compressive strength as a function of the
snap-fit structures tl 2 ratio and relative density are shown in
Fig. 14(a) and (b). The unit cell data is compared with both theDFA model and generalized octet-truss lattice model predictions.The trend in the experimental data changed abruptly atq 0:046 as the failure mechanism changes from elastic to inelas-tic buckling of the out-of-plane struts. The measurements are ingood agreement with the generalized octet-truss lattice modelsfor these two mechanisms: at low relative density (q < 0:046),the measurements follow the elastic buckling model. The measure-ments then become consistent with the inelastic buckling modelwhen q > 0:046. Since the Ti6Al4V alloy exhibits low strainhardening, the inelastic buckling model converges rapidly withthe plastic yielding model when q > 0:10. The generalized octet-truss lattice model slightly underestimated the compressivestrength for q > 0:13; consistent with increased node rotationresistance for high t/l ratios. The generalized octet-truss latticemodel assumed pin-joined struts at these nodes, (k = 1). Howeverthe nodes of the stubby struts appear to have a rotational stiffnessk that lies between 1 and 2 for the octet-truss lattice structuresmade here.
Fig. 15 shows the relative (001) in-plane shear strength ofthe shear samples versus their relative density and comparesthem with both the DFA model and the generalized octet-trusslattice model predictions for (a) a = 45 (001) in-plane shearand (b) a a = 0 (001) in-plane shear. Like the compressiveresponses, the experimental data changed abruptly atq 0:046, which is consistent with a change of failure modefrom elastic to inelastic buckling. Again, the DFA model is notable to predict the shear strengths of the snap-fit lattices. Thegeneralized octet-truss lattice model is able to predict the shearstrength of the a = 0 and Type I a = 45 samples: the measure-ments follow the elastic buckling mode at low relative density(q < 0:046), with a transition to the inelastic buckling mode atq 0:046, and to the plastic yielding mode beyond q 0:1.However, the generalized octet-truss lattice model fails to pre-dict the case of a = 45 Type II. The discrepancies again arisefrom the sample edge effect as mentioned above: the out-of-plane edge struts connecting the end nodes suffer minimal axialdeformations, and thus make a negligible contribution to the in-plane shear strength of the core. Since the fraction of out-of-
plane struts that do not suffer an edge effect is 3/4 of the totalpyramidal struts, we estimate that the in-plane shear strengthof the a = 45 Type II cores should be approximately 3/4 thatof a = 45 Type I cores; the measurements are consistent withthis prediction by multiplying 3/4 to the generalized octet-trusslattice model shear strength prediction for a = 45 Type I cores(Fig. 15(c)). Comparison of model results and measurementsindicates that for low aspect ratio octet-truss lattice structures,the in-plane shear strength is sensitive to boundary conditionswhen the edge nodes have insufficient nodal connectivity toinduce strut stretching.
6. Comparisons with competing materials
The measured compressive moduli and strengths of the snap-fitTi6Al4V octet-truss lattices investigated here were included inthe material property charts of Fig. 2. These two maps do not showthe properties of other anisotropic topology cellular structures,which excel in performance under some loading conditions butare inferior in others. The properties of the titanium octet-truss lat-tice are clearly superior to the lattice structures made from invest-ment cast Al7Si0.3Mg (Deshpande et al., 2001), Ti6Al4V, andTi6Al2Sn4Zr2Mo alloys (Li et al., 2008a,b), as well as Ni7Pdeposited via electrodeposition (Torrents et al., 2012), latticesmade from carbon fiber laminate composites (Cheung andGershenfeld, 2013), photosensitive HDDA polymers and vapordeposited alumina (with solid trusses) (Zheng et al., 2014), andare very competitive with the Al2O3-polymer hybrid octet-trusslattices (Bauer et al., 2014).
The Ti6Al4V octet-truss lattices investigated here are morerobust than brittle Al2O3 counterparts, and are expected to retaingood dimensional stability during loading at temperature up toapproximately 400 C. However, a solid truss has a lower secondarea moment than a hollow truss and thus a lower resistance toelastic buckling; the strengths of the titanium octet-truss latticeswith solid trusses loaded in compression are therefore inferior tothe electrodeposited hollow truss alumina and Ni7P octet-trusslattices (Zheng et al., 2014) for densities lower than 0.18 Mg/m3
where the elastic buckling failure mechanism of the solid strutsis dominant (solid model prediction line shown in Fig. 2(b)). How-ever, it is evident that the predicted compressive moduli of thetitanium octet-truss lattices are superior to the hollow truss Ni7P octet-truss lattices (Zheng et al., 2014) and very competitivewith the hollow truss alumina octet-truss lattices (Zheng et al.,2014) at the lower density range (
Fig. 14. Predicted and measured relative compressive strength (normalized by thesolids yield strength) plotted against (a) (t/l)2 and (b) relative density q of the snap-fit structure. Both the DFA model and generalized octet-truss lattice modelpredictions are shown in (a) as a function of strut aspect ratio. Generalized latticemodel is the abbreviation of generalized octet-truss lattice model.
120 L. Dong et al. / International Journal of Solids and Structures 6061 (2015) 107124
3. The moduli and strengths of the manufactured octet-truss lat-tice structures are well predicted by a generalized octet-trusslattice model. However, the (001) in-plane shear moduli andstrengths are sensitive to boundary conditions for small aspectratio octet-truss lattice structures.
4. The Ti6Al4V octet-truss lattices exhibit excellent overallmechanical properties competitive with existing materials andtopologies, and appear to be a promising candidate for hightemperature, sandwich panel and other applications.
Acknowledgments
We are grateful for the support of this work by the DARPAMCMA program (Grant Number W91CRB-10-1-005) managed byDr. Judah Goldwasser.
Appendix A. Modified RambergOsgood fitting
The true tensile stressstrain curve was separated into twoparts and fitted separately.
For r < r0:2, n = 85, E0 = 123 GPa, r0:2 932 MPa, RambergOsgoodfitting
e rE0 0:002 r
r0:2
n
For r > r0:2, a modified RambergOsgood fitting (Rasmussen,2003) was applied by moving both vertical and horizontal axesfrom the origin to a selected point which enabled a smoothtransition between the two fitting curves. This new origin hadcoordinates e1 0:0085, r1 925 MPa, with an initial Youngsmodulus E1 = 9.77 GPa, The fitting coefficients for the modifiedRambergOsgood relation were then n 1:7, eu 0:1105,ru 1110 MPa, with
e e1 r r1
E1 eu e1
ru r1E1
r r1ru r1
n
Appendix B. Generalized octet-truss lattice model
B.1. Compression
B.1.1. Compressive modulusConsider an edge clamped out-of-plane strut of the octahedral
cell with length l and square cross section of side length t as shownin Fig. A1(a). During free compression, both ends of an out-of-planestrut are able to move due to the Poisson effect of the octahedralcell. Fig. A1 illustrates the deformation behavior of an end clampedout-of-plane strut when the octahedral cell is under free compres-sion. The corresponding free body diagram of such a strut is shownin Fig. A1(b). With an imposed displacement at one end along zdirection denoted as dzz, the lateral displacement at the other endalong x direction denoted as dxx, the axial force FA and shear forceFS in the strut are given by elementary beam theory
FA Est2dzz sin x dxx cos x
lA-1a
FS 12EsIdzz cos x dxx sinx
l3A-1b
where Es is the Youngs modulus of the solid material, x is strutinclined angle (=45), I is the second moment of area of the strutcross section given by I = t4/12 for square cross section of sidelength t. The total applied force, Fstrut, on such a single strut in thez direction follows as
Fstrut FA sinx FS cos x A-2a
Eq. (A-2a) applies for fixed-end (built-in) struts (k = 2); for pin-joined struts (k = 1), the contribution to the stiffness due to thebending of the struts is negligible, and Eq. (A-2a) reduces to
Fstrut FA sinx Est2dzz dxx
2lA-2b
In the case of pin-joined struts, the basic force analysis showedthat the lateral displacement dxx is related to the vertical displace-ment dzz by
dxx 13
dzz A-3
Therefore, Eq. (A-2b) reduces to
Fstrut FA sinx Est2dzz
3lA-4
Now consider the octahedral cell sketched in Fig. A1(a). Thetotal force, F, applied on the octahedral cell in the z direction isequal to 4Fstrut; stress, rzz and strain, ezz applied to the octahedralcell are related to the force F and displacement dzz via;
rzz FA 4Est
2dzz3lA
A-5
Fig. 15. Predicted and measured relative shear strength for a = 45 plotted against (a) (t/l)2 and (b) relative density q of the snap-fit structure. Both the DFA model andgeneralized octet-truss lattice model predictions are shown in (a) and (c). Analogous results for loading at a = 0 are shown in (c) and (d). Generalized lattice model is theabbreviation of generalized octet-truss lattice model.
L. Dong et al. / International Journal of Solids and Structures 6061 (2015) 107124 121
and
ezz 2dzzH
A-6
where H is octahedral cell height H 2l sinx h 2htab, A is
cross-sectional area (A 2l cos xbcffiffi2p
2), as shown in Fig. 4(c). The
effective Youngs modulus Ezz of the octahedral cell in free compres-sion is then given by;
Ezz rzzezz 2t
2
3HlA
Es A-7
Eq. (A-7) can be expressed in terms of the relative compressivemodulus as
EzzEs 2t
2
3HlA Kel
HlA
A-8
with Kel 23 t2.
B.1.2. Compressive strengthEq. (A-5) gives the compressive stress rzz applied to the octahe-
dral cell in the z direction; the corresponding axial stress rA in anout-of-plane strut is given by
rA Esdzz dxxffiffiffi
2p
l
ffiffiffi2p
Esdzz3l
A-9
Therefore, the stress applied to the octahedral cell, rzz, can beexpressed in terms of the axial stress, rA, in an out-of-plane strut;
rzz 2ffiffiffi2p
t2
ArA A-10
The out-of-plane strut can support load until its collapsestrength rc is achieved. Therefore, the lattice strength is given by
rpkzz 2ffiffiffi2p
t2
Arc A-11
Eq. (A-11) can be expressed in terms of the relative compressivestrength of the lattice as
rpkzzrys 2
ffiffiffi2p
t2rcrysA
KrrcA
A-12
where Kr is a constant =2ffiffi2p
t2rys ; rys is the yield strength of the solid
material.
B.2. (001) in-plane shear
B.2.1. (001) in-plane shear modulusConsider the octahedral cell sketched in Fig. A1(a) with an
applied in-plane shear displacement d0 applied to the top node ofthe octahedral cell in the direction defined by an angle a(0 6 a 6 45, due to symmetry). Such a displacement can beresolved into two components perpendicular to each other as;
d0x d0 cos a A-13a
and
d0y d0 sin a A-13b
Fig. 16. Material property charts showing (a) the shear modulus and (b) the shearstrength experimental data (45 Type I) and model predictions (solid curves) for thesnap-fit Ti6Al4V octet lattices investigated here. The shear properties of polymerand metal foams and several solid materials are also shown for comparison.
122 L. Dong et al. / International Journal of Solids and Structures 6061 (2015) 107124
Fig. A1(c) shows an edge clamped strut with length of l and sidelength t (width equals to length) and its free body diagram repre-senting a single out-of-plane strut of an octahedral cell. Symmetry
Fig. A1. Sketch of the deformation of a single out-of-plane strut under uniaxial compressiand shear forces present when the unit cell is under uniaxial free compression (b) or in
condition dictates that displacements and rotations of nodes apartfrom the top and bottom shown in Fig. A1(a) are constrained. Theaxial and shear displacements applied to the strut within the planeparallel to the d0x direction are;
d0a d0x cos x A-14a
and
d0s d0x sin x A-14b
with such a strut subjected to either compression or tensile dis-placement. According to elementary beam theory, the axial andshear forces in such a strut are given by
F 0A Est2d0x cos x
lA-15a
and
F 0S 12EsId0x sin x
l3A-15b
The total force applied along the d0x direction of a unit cell is
F 0x 2 F0A cos x F
0S sin x
Est
2d0xl
1 tl
2" #A-16a
The force applied along the d0y direction is;
F 0y 2 F0A cos x F
0S sin x
Est2d0y
l1 t
l
2" #A-16b
It is noted that Eq. (A-16) was derived assuming fixed-end(built-in) struts (k = 2); for pin-joined struts (k = 1), the contribu-tion to the stiffness due to the bending of the struts is negligible,
and the t=l2 related terms (i.e., F 0S terms) in Eq. (A-16) disappear,and the total shear force, F 0, applied on the unit cell is then
F 0 ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiF 02x F
02y
q Est
2d0
lA-17
The total shear stress applied on the unit cell is thus
s F0
A Est
2d0
AlA-18
The shear strain
c 2d0
HA-19
on and in shear. Free body diagram for such a strut showing the combination of axialshear (c).
L. Dong et al. / International Journal of Solids and Structures 6061 (2015) 107124 123
Therefore, the shear modulus of the lattice is
G sc t
2H2Al
Es A-20
Eq. (A-20) can be expressed in terms of the (001) in-plane rela-tive shear modulus as
GEs t
2H2Al Kel
HAl
A-21
with Kel 12 t2.
B.2.2. (001) in-plane shear strengthEq. (A-18)represents the total shear stress applied on the unit
cell ((001) in-plane shear). The axial stress in an out-of-plane strutis given by
rA Esd
0 cos affiffiffi2p
lA-22
Therefore, the (001) in-plane shear stress applied to the octahe-dral cell, s, can be expressed in terms of the axial stress, rA, in anout-of-plane strut;
s rAffiffiffi2p
t2
A cos aA-23
The out-of-plane strut can support load until its collapsestrength rc is achieved. Therefore, the lattice shear strength isgiven by
spk rcffiffiffi2p
t2
A cos aA-24
Eq. (A-24) can be expressed in terms of the (001) in-plane rela-tive shear strength of the lattice as
spkrys
ffiffiffi2p
t2
rys cos arcA Ks
rcA
A-25
where Ks is a constant =ffiffi2p
t2rys cos a.
Appendix C. Brazed joint minimum shear strength prediction
For the octahedral cell shown in Fig. 4(c), the contact area ofpyramidal struts with the intermediate layer at a node is given by;
Anode 2bt t2 A-26
Eq. (A-24) indicates that the peak shear force applied to theoctahedral cell is
spkA rcffiffiffi2p
t2
cos aA-27
To avoid node shear fracture dominated behavior, the brazedjoint requires a sufficient shear strength to prevent node shearfracture prior to the attainment of peak stress under (001) in-plane shear. The minimum shear strength required for the brazedjoint, sbraze is therefore,
sbraze Anode P spkA rcffiffiffi2p
t2
cos aA-28
When a 45,
sbraze P rc2t
2b t A-29
If we conservatively take rc 1:1 GPa (see Fig. 9) as the col-lapse strength of a single solid strut (an upper limit for rc),sbraze P 440 MPa. The measured shear strength of the brazed joint
was 450 MPa; just sufficient to prevent node shear fracture becom-ing the dominate failure mechanism for the shear samplesmanufactured and tested here.
It is also noted that, the node area (2bt t2) used for the calcu-lation above is an overly conservative estimate of brazed joint sur-face area (i.e. the trusses contact area) at a node. In reality, thebrazed joint surface area at a node is larger 6bt t2, as the inter-mediate layer struts also meet the pyramidal struts at this node.
References
Adams, D.F., 2007. Shear testing of sandwich panel core materials. High-Performance Compos. 15, 89.
Ashby, M.F., 2000. Metal Foams: A Design Guide. Butterworth-Heinemann.Bauer, Jens, Hengsbach, Stefan, Tesari, Iwiza, Schwaiger, Ruth, Kraft, Oliver, 2014.
High-strength cellular ceramic composites with 3D microarchitecture. Proc.Natl. Acad. Sci. 111, 24532458.
Bitzer, T., 1997. Honeycomb technology. Chapman & Hall, London.Boomsma, K., Poulikakos, D., Zwick, F., 2003. Metal foams as compact high
performance heat exchangers. Mech. Mater. 35, 11611176.Botstein, O., Rabinkin, A., 1994. Brazing of titanium-based alloys with amorphous
25wt.% Ti-25wt.% Zr-50wt.% Cu filler metal. Mater. Sci. Eng., A 188, 305315.Boyer, R.R., Briggs, R.D., 2005. The use of b titanium alloys in the aerospace industry.
J. Mater. Eng. Perform. 14 (6), 681685.Boyer, R., Collings, E.W. (Eds.), 1993. Materials Properties Handbook: Titanium
Alloys. ASM International.Brewer, W.D., Bird, R.K., Terryl, A.W., 1998. Titanium alloys and processing for high
speed aircraft. Mater. Sci. Eng., A 243, 299304.Cheung, K.C., Gershenfeld, N., 2013. Reversibly assembled cellular composite
materials. Science 341, 12191221.Chu, J., Engelbrecht, S., Graf, G., Rosen, D.W., 2010. A comparison of synthesis
methods for cellular structures with application to additive manufacturing.Rapid Prototyping J. 16, 275283.
Couper, J.R., Penney, W.R., Fair, J.R., 2009. Chemical Process Equipment revised 2ndEdition: Selection and Design, second ed. Gulf Professional Publishing.
Deshpande, V.S., Ashby, M.F., Fleck, N.A., 2001. Foam topology: bending versusstretching dominated architectures. Acta Mater. 49, 10351040.
Deshpande, V.S., Fleck, N.A., Ashby, M.F., 2001. Effective properties of the octet-trusslattice material. J. Mech. Phys. Solids 49, 17471769.
Dharmasena, Kumar P., Wadley, Haydn N.G., Xue, Zhenyu, Hutchinson, John W.,2008. Mechanical response of metallic honeycomb sandwich panel structuresto high-intensity dynamic loading. Int. J. Impact Eng. 35, 10631074.
Donachie, M.J., 2000. Titanium: A Technical Guide. ASM International.Finnegan, K., Kooistra, G., Wadley, H.N., Deshpande, V.S., 2007. The compressive
response of carbon fiber composite pyramidal truss sandwich cores. Int. J.Mater. Res. 98, 12641272.
Froes, F.H., Friedrich, H., Kiese, J., Bergoint, D., 2004. Titanium in the familyautomobile: the cost challenge. JOM 56, 4044.
Fuller, R.B., 1961, Octet Truss. U.S. Patent No. 2,986,241.Gere, J.M., Timoshenko, S.P., 1984. Mechanics of Materials. PWS Engineering,
Boston.Gibson, L.J., Ashby, M.F., 1999. Cellular Solids: Structure and Properties. Cambridge
University Press.Gorynin, I.V., 1999. Titanium alloys for marine application. Mater. Sci. Eng., A 263,
112116.Holloman, Ryan, Deshpande, Vikram, Hanssen, Arve, Fleming, Katherine, Scully,
John, Wadley, Haydn, 2013. Tubular aluminum cellular structures: fabricationand mechanical response. J. Mech. Mater. Struct. 8, 6594.
Kooistra, Gregory W., Deshpande, Vikram S., Wadley, Haydn N.G., 2004.Compressive behavior of age hardenable tetrahedral lattice truss structuresmade from aluminium. Acta Mater. 52, 42294237.
Kooistra, Gregory W., Wadley, Haydn N.G., 2007. Lattice truss structures fromexpanded metal sheet. Mater. Des. 28, 507514.
Kulekci, M.K., 2008. Magnesium and its alloys applications in automotive industry.Int. J. Adv. Manuf. Technol. 39, 851865.
Lee, Yong-Hyun, Lee, Byung-Kon, Jeon, Insu, Kang, Ki-Ju, 2007. Wire-woven bulkKagome truss cores. Acta Mater. 55, 60846094.
Li, Q., Chen, Y.C.E.Y., Douglas, R.B., Dunand, D.C., 2008a. Mechanical properties ofcast Ti6Al4V lattice block structures. Metall. Mater. Trans. A 39, 441449.
Li, Q., Chen, Y.C.E.Y., Douglas, R.B., Dunand, D.C., 2008b. Mechanical properties ofcast Ti6Al2Sn4Zr2Mo lattice block structures. Adv. Eng. Mater. 10, 939942.
Lim, Ji-Hyun, Kang, Ki-Ju, 2006. Mechanical behavior of sandwich panels withtetrahedral and Kagome truss cores fabricated from wires. Int. J. Solids Struct.43, 52285246.
Lu, T.J., Stone, H.A., Ashby, M.F., 1998. Heat transfer in open-cell metal foams. ActaMater. 46, 36193635.
Lugscheider, E., Broich, U., 1995 May. Mechanical properties of high-temperaturebrazed titanium materials, American Welding Society, Welding ResearchSupplement, pp. 169176.
Onzawa, T., Suzumura, A., Ko, M.W., 1990. Brazing of titanium using low-melting-point Ti-based filler metals. Weld. J. 69, 462467.
http://refhub.elsevier.com/S0020-7683(15)00066-9/h0005http://refhub.elsevier.com/S0020-7683(15)00066-9/h0005http://refhub.elsevier.com/S0020-7683(15)00066-9/h0010http://refhub.elsevier.com/S0020-7683(15)00066-9/h0015http://refhub.elsevier.com/S0020-7683(15)00066-9/h0015http://refhub.elsevier.com/S0020-7683(15)00066-9/h0015http://refhub.elsevier.com/S0020-7683(15)00066-9/h0020http://refhub.elsevier.com/S0020-7683(15)00066-9/h0025http://refhub.elsevier.com/S0020-7683(15)00066-9/h0025http://refhub.elsevier.com/S0020-7683(15)00066-9/h0030http://refhub.elsevier.com/S0020-7683(15)00066-9/h0030http://refhub.elsevier.com/S0020-7683(15)00066-9/h0035http://refhub.elsevier.com/S0020-7683(15)00066-9/h0035http://refhub.elsevier.com/S0020-7683(15)00066-9/h0040http://refhub.elsevier.com/S0020-7683(15)00066-9/h0040http://refhub.elsevier.com/S0020-7683(15)00066-9/h0045http://refhub.elsevier.com/S0020-7683(15)00066-9/h0045http://refhub.elsevier.com/S0020-7683(15)00066-9/h0050http://refhub.elsevier.com/S0020-7683(15)00066-9/h0050http://refhub.elsevier.com/S0020-7683(15)00066-9/h0055http://refhub.elsevier.com/S0020-7683(15)00066-9/h0055http://refhub.elsevier.com/S0020-7683(15)00066-9/h0055http://refhub.elsevier.com/S0020-7683(15)00066-9/h0060http://refhub.elsevier.com/S0020-7683(15)00066-9/h0060http://refhub.elsevier.com/S0020-7683(15)00066-9/h0065http://refhub.elsevier.com/S0020-7683(15)00066-9/h0065http://refhub.elsevier.com/S0020-7683(15)00066-9/h0070http://refhub.elsevier.com/S0020-7683(15)00066-9/h0070http://refhub.elsevier.com/S0020-7683(15)00066-9/h0075http://refhub.elsevier.com/S0020-7683(15)00066-9/h0075http://refhub.elsevier.com/S0020-7683(15)00066-9/h0075http://refhub.elsevier.com/S0020-7683(15)00066-9/h0080http://refhub.elsevier.com/S0020-7683(15)00066-9/h0085http://refhub.elsevier.com/S0020-7683(15)00066-9/h0085http://refhub.elsevier.com/S0020-7683(15)00066-9/h0085http://refhub.elsevier.com/S0020-7683(15)00066-9/h0090http://refhub.elsevier.com/S0020-7683(15)00066-9/h0090http://refhub.elsevier.com/S0020-7683(15)00066-9/h0100http://refhub.elsevier.com/S0020-7683(15)00066-9/h0100http://refhub.elsevier.com/S0020-7683(15)00066-9/h0105http://refhub.elsevier.com/S0020-7683(15)00066-9/h0105http://refhub.elsevier.com/S0020-7683(15)00066-9/h0110http://refhub.elsevier.com/S0020-7683(15)00066-9/h0110http://refhub.elsevier.com/S0020-7683(15)00066-9/h0115http://refhub.elsevier.com/S0020-7683(15)00066-9/h0115http://refhub.elsevier.com/S0020-7683(15)00066-9/h0115http://refhub.elsevier.com/S0020-7683(15)00066-9/h0120http://refhub.elsevier.com/S0020-7683(15)00066-9/h0120http://refhub.elsevier.com/S0020-7683(15)00066-9/h0120http://refhub.elsevier.com/S0020-7683(15)00066-9/h0125http://refhub.elsevier.com/S0020-7683(15)00066-9/h0125http://refhub.elsevier.com/S0020-7683(15)00066-9/h0130http://refhub.elsevier.com/S0020-7683(15)00066-9/h0130http://refhub.elsevier.com/S0020-7683(15)00066-9/h0135http://refhub.elsevier.com/S0020-7683(15)00066-9/h0135http://refhub.elsevier.com/S0020-7683(15)00066-9/h0140http://refhub.elsevier.com/S0020-7683(15)00066-9/h0140http://refhub.elsevier.com/S0020-7683(15)00066-9/h0145http://refhub.elsevier.com/S0020-7683(15)00066-9/h0145http://refhub.elsevier.com/S0020-7683(15)00066-9/h0145http://refhub.elsevier.com/S0020-7683(15)00066-9/h0150http://refhub.elsevier.com/S0020-7683(15)00066-9/h0150http://refhub.elsevier.com/S0020-7683(15)00066-9/h0150http://refhub.elsevier.com/S0020-7683(15)00066-9/h0155http://refhub.elsevier.com/S0020-7683(15)00066-9/h0155http://refhub.elsevier.com/S0020-7683(15)00066-9/h0165http://refhub.elsevier.com/S0020-7683(15)00066-9/h0165
124 L. Dong et al. / International Journal of Solids and Structures 6061 (2015) 107124
Park, J.S., Joo, J.H., Lee, B.C., Kang, K.J., 2011. Mechanical behaviour of tube-wovenKagome truss cores under compression. Int. J. Mech. Sci. 53 (1), 6573.
Queheillalt, Douglas T., Wadley, Haydn N.G., 2005. Pyramidal lattice truss structureswith hollow trusses. Mater. Sci. Eng., A 397, 132137.
Queheillalt, Douglas T., Murty, Yellapu, Wadley, Haydn N.G., 2008. Mechanicalproperties of an extruded pyramidal lattice truss sandwich structure. ScriptaMater. 58, 7679.
Rasmussen, K.J.R., 2003. Full range stress strain curves for stainless steel alloys. J.Constr. Steel Res. 59, 4761.
Ritchie, R.O., Boyce, B.L., Campbell, J.P., Roder, O., Thompson, A.W., Milligan, W.W.,1999. Thresholds for high-cycle fatigue in a turbine engine Ti6Al4V alloy. Int.J. Fatigue 21, 653662.
Rosen, D.W., 2007. Computer-aided design for additive manufacturing of cellularstructures. Comput.-Aided Des. Appl. 4, 585594.
Russell, Benjamin, Deshpande, Vikram, Wadley, Haydn, 2008. Quasistaticdeformation and failure modes of composite square honeycombs. J. Mech.Mater. Struct. 3, 13151340.
SanMarchi, C., Mortensen, A., 2002. Handbook of Cellular Metals. Wiley-VCH Verlag,Weinheim Germany.
Shanley, F.R., 1967. Mechanics of Materials. McGraw-Hill, New York.
Sypeck, David J., Wadley, Haydn N.G., 2002. Cellular metal truss core sandwichstructures. Adv. Eng. Mater. 4, 759764.
Torrents, A., Schaedler, T.A., Jacobsen, A.J., Carter, W.B., Valdevit, L., 2012.Characterization of nickel-based microlattice materials with structural hierarchyfrom the nanometer to the millimeter scale. Acta Mater. 60, 35113523.
Wadley, Haydn N.G., Fleck, Norman A., Evans, Anthony G., 2003. Fabrication andstructural performance of periodic cellular metal sandwich structures. Compos.Sci. Technol. 63, 23312343.
Wadley, Haydn N.G., 2006. Multifunctional periodic cellular metals. Philos. Trans. R.Soc. A: Math. Phys. Eng. Sci. 364, 3168.
Wang, J., Evans, A.G., Dharmasena, K., Wadley, H.N.G., 2003. On the performance oftruss panels with Kagome cores. Int. J. Solids Struct. 40, 69816988.
Williams, C.B., Cochran, J.K., Rosen, D.W., 2011. Additive manufacturing of metalliccellular materials via three-dimensional printing. Int. J. Adv. Manuf. Technol. 53,231239.
Ye, H., 2003. An overview of the development of AlSi-alloy based material forengine applications. J. Mater. Eng. Perform. 12, 288297.
Zheng, Xiaoyu, Lee, Howon, Weisgraber, Todd H., Shusteff, Maxim, Deotte, Joshua R.,Duoss, Eric, Kuntz, Joshua D., et al., 2014. Ultra-light, ultra-stiff mechanicalmetamaterials. Science 344, 13731377.
http://refhub.elsevier.com/S0020-7683(15)00066-9/h0170http://refhub.elsevier.com/S0020-7683(15)00066-9/h0170http://refhub.elsevier.com/S0020-7683(15)00066-9/h0175http://refhub.elsevier.com/S0020-7683(15)00066-9/h0175http://refhub.elsevier.com/S0020-7683(15)00066-9/h0180http://refhub.elsevier.com/S0020-7683(15)00066-9/h0180http://refhub.elsevier.com/S0020-7683(15)00066-9/h0180http://refhub.elsevier.com/S0020-7683(15)00066-9/h0185http://refhub.elsevier.com/S0020-7683(15)00066-9/h0185http://refhub.elsevier.com/S0020-7683(15)00066-9/h0190http://refhub.elsevier.com/S0020-7683(15)00066-9/h0190http://refhub.elsevier.com/S0020-7683(15)00066-9/h0190http://refhub.elsevier.com/S0020-7683(15)00066-9/h0195http://refhub.elsevier.com/S0020-7683(15)00066-9/h0195http://refhub.elsevier.com/S0020-7683(15)00066-9/h0200http://refhub.elsevier.com/S0020-7683(15)00066-9/h0200http://refhub.elsevier.com/S0020-7683(15)00066-9/h0200http://refhub.elsevier.com/S0020-7683(15)00066-9/h0205http://refhub.elsevier.com/S0020-7683(15)00066-9/h0205http://refhub.elsevier.com/S0020-7683(15)00066-9/h0210http://refhub.elsevier.com/S0020-7683(15)00066-9/h0215http://refhub.elsevier.com/S0020-7683(15)00066-9/h0215http://refhub.elsevier.com/S0020-7683(15)00066-9/h0220http://refhub.elsevier.com/S0020-7683(15)00066-9/h0220http://refhub.elsevier.com/S0020-7683(15)00066-9/h0220http://refhub.elsevier.com/S0020-7683(15)00066-9/h0225http://refhub.elsevier.com/S0020-7683(15)00066-9/h0225http://refhub.elsevier.com/S0020-7683(15)00066-9/h0225http://refhub.elsevier.com/S0020-7683(15)00066-9/h0230http://refhub.elsevier.com/S0020-7683(15)00066-9/h0230http://refhub.elsevier.com/S0020-7683(15)00066-9/h0235http://refhub.elsevier.com/S0020-7683(15)00066-9/h0235http://refhub.elsevier.com/S0020-7683(15)00066-9/h0240http://refhub.elsevier.com/S0020-7683(15)00066-9/h0240http://refhub.elsevier.com/S0020-7683(15)00066-9/h0240http://refhub.elsevier.com/S0020-7683(15)00066-9/h0245http://refhub.elsevier.com/S0020-7683(15)00066-9/h0245http://refhub.elsevier.com/S0020-7683(15)00066-9/h0250http://refhub.elsevier.com/S0020-7683(15)00066-9/h0250http://refhub.elsevier.com/S0020-7683(15)00066-9/h0250
Mechanical response of Ti6Al4V octet-truss lattice structures1 Introduction2 Lattice fabrication, relative density and solid material properties2.1 Lattice fabrication2.2 Relative density2.3 Solid material characterization
3 Compression and shear responses3.1 Compression results3.2 Shear results
4 DFA and generalized models for octet-truss lattice4.1 Stiffness predictions4.2 Strength predictions4.2.1 Compressive strength4.2.2 The (001) in-plane shear strength
5 Comparison of predictions with measurements6 Comparisons with competing materials7 ConclusionsAcknowledgmentsAppendix A Modified RambergOsgood fittingAppendix B Generalized octet-truss lattice modelB.1 CompressionB.1.1 Compressive modulusB.1.2 Compressive strength
B.2 (001) in-plane shearB.2.1 (001) in-plane shear modulusB.2.2 (001) in-plane shear strength
Appendix C Brazed joint minimum shear strength predictionReferences